Incommensurately modulated ordering of tetrahedral chains in Ca~2~Fe~2~O~5~ at elevated temperatures
Krüger, Hannes; Kahlenberg, Volker; Acta Crystallographica Section B 61 (2005) 656–662; doi:10.1107/S0108768105026480

data_1101062
_publ_section_title
;
 Incommensurately modulated ordering of tetrahedral chains in
 Ca~2~Fe~2~O~5~ at elevated temperatures
;
_journal_coeditor_code           SN5023
_journal_issue                   06
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              656
_journal_page_last               662
_journal_paper_doi               10.1107/S0108768105026480
_journal_volume                  61
_journal_year                    2005
_chemical_formula_sum            'Ca2 Fe2 O5'
_chemical_formula_weight         271.8
_chemical_name_systematic        ' ?'
_space_group_ssg_name            Imma(00\g)s00
_symmetry_cell_setting           orthorhombic
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.4931(12)
_cell_length_b                   15.038(3)
_cell_length_c                   5.6511(11)
_cell_measurement_reflns_used    2473
_cell_measurement_temperature    1100
_cell_measurement_theta_max      29.54
_cell_measurement_theta_min      2.71
_cell_modulation_dimension       1
_cell_volume                     466.81(17)
_computing_cell_refinement       'STOE X-AREA'
_computing_data_collection       'STOE X-AREA'
_computing_data_reduction        'STOE X-RED'
_computing_publication_material  '(Jana2000; Petricek and Dusek, 2000)'
_computing_structure_refinement  '(Jana2000; Petricek and Dusek, 2000)'
_diffrn_ambient_temperature      1100
_diffrn_detector                 'image plate (34 cm diameter)'
_diffrn_detector_area_resol_mean 6.67
_diffrn_detector_type            STOE
_diffrn_measured_fraction_theta_full 0.98
_diffrn_measurement_details      ' 120 frames, detector distance = 100 mm'
_diffrn_measurement_device       '2-circle goniometer'
_diffrn_measurement_device_type  'STOE IPDS 2'
_diffrn_measurement_method       'rotation method'
_diffrn_radiation_collimation    '0.5 mm diameter, multiple pinhole'
_diffrn_radiation_monochromator  'plane graphite'
_diffrn_radiation_polarisn_norm  0
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0586
_diffrn_reflns_av_sigmaI/netI    0.0112
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_index_m_1_max 1
_diffrn_reflns_limit_index_m_1_min -1
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_limit_l_min       -7
_diffrn_reflns_number            6040
_diffrn_reflns_theta_full        29.31
_diffrn_reflns_theta_max         29.31
_diffrn_reflns_theta_min         2.71
_diffrn_source
'sealed X-ray tube, 12 x 0.4 mm long-fine focus'
_diffrn_source_current           40
_diffrn_source_power             2.00
_diffrn_source_voltage           50
_exptl_absorpt_coefficient_mu    8.331
_exptl_absorpt_correction_T_max  0.6093
_exptl_absorpt_correction_T_min  0.3086
_exptl_absorpt_correction_type   integration
_exptl_absorpt_process_details   'STOE X-RED'
_exptl_crystal_colour            reddish-brown
_exptl_crystal_density_diffrn    3.8670
_exptl_crystal_description       plate
_exptl_crystal_F_000             528
_exptl_crystal_size_max          0.18
_exptl_crystal_size_mid          0.18
_exptl_crystal_size_min          0.06
_refine_diff_density_max         1.29
_refine_diff_density_min         -1.96
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_gt    3.15
_refine_ls_goodness_of_fit_ref   2.91
_refine_ls_number_parameters     43
_refine_ls_number_reflns         934
_refine_ls_R_factor_all          0.0667
_refine_ls_R_factor_gt           0.0530
_refine_ls_shift/su_max          0.0010
_refine_ls_shift/su_mean         0.0001
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/(\s^2^(F)+0.0001F^2^)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0535
_refine_ls_wR_factor_ref         0.0550
_reflns_number_gt                759
_reflns_number_total             934
_reflns_threshold_expression     I>3\s(I)
_cod_data_source_file            sn5023.cif
_cod_data_source_block           I
_cod_original_cell_volume        466.79(17)
_cod_database_code               1101062